#------------------------------------------------------------------------------
#$Date: 2016-03-26 17:01:19 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180368 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/37/7203775.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7203775
loop_
_publ_author_name
'León-Reina, Laura'
'Losilla, Enrique R.'
'Martínez-Lara, Maria'
'Bruque, Sebastián'
'Llobet, Anna'
'Sheptyakov, Denis V.'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Interstitial oxygen in oxygen-stoichiometric apatites
;
_journal_issue                   25
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2489
_journal_paper_doi               10.1039/b503374h
_journal_volume                  15
_journal_year                    2005
_chemical_formula_sum            'La1.33 O4.33 Si Sr0.33'
_chemical_formula_weight         311.83
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_audit_creation_date             2004-06-11T10:37
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2004-06-11T10:37 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.71191(8)
_cell_length_b                   9.71191
_cell_length_c                   7.23956(7)
_cell_volume                     591.360(8)
_computing_structure_refinement  GSAS
_pd_block_id
2004-06-11T10:37|SR2SI_NPD_RX|La8Sr2Si6O26|Overall
_pd_phase_name
'from C:/RIETVELD/Apatito/SINQ_02/La9.55Si/La955Si6_RT/LA955SI.EXP'
_pd_proc_ls_prof_R_factor        0.0403
_pd_proc_ls_prof_wR_factor       0.0231
_refine_ls_goodness_of_fit_all   1.70
_refine_ls_matrix_type           full
_refine_ls_number_parameters     103
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.06
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            b503374h.txt
_cod_data_source_block           SR2SI_NPD_RX_publ
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (817
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (180 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        591.36029
_cod_database_code               7203775
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.23242(7) -0.01319(8) 0.25 0.8 Uani 0.00298 6
LA La2 0.3333 0.6667 -0.00060(13) 0.8 Uani 0.00897 4
SI SI 0.40032(15) 0.37000(14) 0.25 1.0 Uani 0.00359 6
O O1 0.32297(13) 0.48432(14) 0.25 1.0 Uani 0.00867 6
O O2 0.59378(11) 0.47133(13) 0.25 1.0 Uani 0.00772 6
O O3 0.34192(11) 0.25364(10) 0.07004(8) 1.0 Uani 0.01147 12
O O4 0.0 0.0 0.25 1.024(7) Uani 0.01535 2
SR Sr1 0.23242(7) -0.01319(8) 0.25 0.2 Uani 0.00298 6
SR Sr2 0.33333 0.66667 -0.00060(13) 0.2 Uani 0.00897 4
O O5 0.005 0.242 0.61 -0.0039(11) Uiso 0.025 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 8.0
SI 6.0
O 26.0
SR 2.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 99.86(4) 5_555 . 3_655 n
O1 La1 O3 148.079(17) 5_555 . 1_555 n
O1 La1 O3 71.748(22) 5_555 . 6_555 n
O1 La1 O3 71.748(22) 5_555 . -3_555 n
O1 La1 O3 148.079(17) 5_555 . -4_556 n
O1 La1 O4 110.087(30) 5_555 . 1_555 n
O1 La1 Sr1 140.087(30) 5_555 . 3_555 n
O1 La1 Sr1 80.087(30) 5_555 . 5_555 n
O1 La1 O5 53.370(21) 5_555 . 4_554 n
O1 La1 O5 91.414(14) 5_555 . 5_555 n
O1 La1 O5 154.727(14) 5_555 . 6_554 n
O1 La1 O5 53.370(21) 5_555 . -1_556 n
O1 La1 O5 91.414(14) 5_555 . -2_556 n
O1 La1 O5 154.727(14) 5_555 . -3_556 n
O2 La1 O3 71.660(31) 3_655 . 1_555 n
O2 La1 O3 84.917(25) 3_655 . 6_555 n
O2 La1 O3 84.917(25) 3_655 . -3_555 n
O2 La1 O3 71.660(31) 3_655 . -4_556 n
O2 La1 O4 150.05(4) 3_655 . 1_555 n
O2 La1 Sr1 120.05(4) 3_655 . 3_555 n
O2 La1 Sr1 179.9557 3_655 . 5_555 n
O2 La1 O5 141.517(26) 3_655 . 4_554 n
O2 La1 O5 89.216(13) 3_655 . 5_555 n
O2 La1 O5 90.782(29) 3_655 . 6_554 n
O2 La1 O5 141.517(26) 3_655 . -1_556 n
O2 La1 O5 89.216(13) 3_655 . -2_556 n
O2 La1 O5 90.782(29) 3_655 . -3_556 n
O3 La1 O3 135.269(34) 1_555 . 6_555 n
O3 La1 O3 76.800(16) 1_555 . -3_555 n
O3 La1 O3 60.008(32) 1_555 . -4_556 n
O3 La1 O4 82.522(24) 1_555 . 1_555 n
O3 La1 Sr1 57.263(24) 1_555 . 3_555 n
O3 La1 Sr1 108.383(23) 1_555 . 5_555 n
O3 La1 O5 114.889(20) 1_555 . 4_554 n
O3 La1 O5 118.509(26) 1_555 . 5_555 n
O3 La1 O5 20.974(18) 1_555 . 6_554 n
O3 La1 O5 146.031(29) 1_555 . -1_556 n
O3 La1 O5 58.501(15) 1_555 . -2_556 n
O3 La1 O5 57.144(20) 1_555 . -3_556 n
O3 La1 O3 139.65(5) 6_555 . -3_555 n
O3 La1 O3 76.800(16) 6_555 . -4_556 n
O3 La1 O4 104.073(25) 6_555 . 1_555 n
O3 La1 Sr1 109.443(24) 6_555 . 3_555 n
O3 La1 Sr1 95.066(27) 6_555 . 5_555 n
O3 La1 O5 107.232(28) 6_555 . 4_554 n
O3 La1 O5 21.254(19) 6_555 . 5_555 n
O3 La1 O5 132.460(26) 6_555 . 6_554 n
O3 La1 O5 61.933(21) 6_555 . -1_556 n
O3 La1 O5 160.850(32) 6_555 . -2_556 n
O3 La1 O5 86.604(20) 6_555 . -3_556 n
O3 La1 O3 135.268(34) -3_555 . -4_556 n
O3 La1 O4 104.073(25) -3_555 . 1_555 n
O3 La1 Sr1 109.443(24) -3_555 . 3_555 n
O3 La1 Sr1 95.066(27) -3_555 . 5_555 n
O3 La1 O5 61.933(21) -3_555 . 4_554 n
O3 La1 O5 160.850(32) -3_555 . 5_555 n
O3 La1 O5 86.604(20) -3_555 . 6_554 n
O3 La1 O5 107.232(28) -3_555 . -1_556 n
O3 La1 O5 21.254(19) -3_555 . -2_556 n
O3 La1 O5 132.460(26) -3_555 . -3_556 n
O3 La1 O4 82.522(24) -4_556 . 1_555 n
O3 La1 Sr1 57.263(24) -4_556 . 3_555 n
O3 La1 Sr1 108.383(23) -4_556 . 5_555 n
O3 La1 O5 146.031(29) -4_556 . 4_554 n
O3 La1 O5 58.501(15) -4_556 . 5_555 n
O3 La1 O5 57.144(20) -4_556 . 6_554 n
O3 La1 O5 114.889(20) -4_556 . -1_556 n
O3 La1 O5 118.509(26) -4_556 . -2_556 n
O3 La1 O5 20.974(18) -4_556 . -3_556 n
O4 La1 Sr1 30.0 1_555 . 3_555 n
O4 La1 Sr1 30.0 1_555 . 5_555 n
O4 La1 O5 63.649(14) 1_555 . 4_554 n
O4 La1 O5 90.031(12) 1_555 . 5_555 n
O4 La1 O5 61.885(14) 1_555 . 6_554 n
O4 La1 O5 63.649(14) 1_555 . -1_556 n
O4 La1 O5 90.031(12) 1_555 . -2_556 n
O4 La1 O5 61.885(14) 1_555 . -3_556 n
Sr1 La1 Sr1 60.0 3_555 . 5_555 n
Sr1 La1 O5 90.825(13) 3_555 . 4_554 n
Sr1 La1 O5 89.269(13) 3_555 . 5_555 n
Sr1 La1 O5 36.547(13) 3_555 . 6_554 n
Sr1 La1 O5 90.825(13) 3_555 . -1_556 n
Sr1 La1 O5 89.269(13) 3_555 . -2_556 n
Sr1 La1 O5 36.547(13) 3_555 . -3_556 n
Sr1 La1 O5 38.445(14) 5_555 . 4_554 n
Sr1 La1 O5 90.785(13) 5_555 . 5_555 n
Sr1 La1 O5 89.264(13) 5_555 . 6_554 n
Sr1 La1 O5 38.445(14) 5_555 . -1_556 n
Sr1 La1 O5 90.785(13) 5_555 . -2_556 n
Sr1 La1 O5 89.264(13) 5_555 . -3_556 n
O5 La1 O5 115.444(20) 4_554 . 5_555 n
O5 La1 O5 105.165(15) 4_554 . 6_554 n
O5 La1 O5 48.212(12) 4_554 . -1_556 n
O5 La1 O5 67.236(8) 4_554 . -2_556 n
O5 La1 O5 125.529(22) 4_554 . -3_556 n
O5 La1 O5 111.738(19) 5_555 . 6_554 n
O5 La1 O5 67.236(8) 5_555 . -1_556 n
O5 La1 O5 176.966(29) 5_555 . -2_556 n
O5 La1 O5 65.689(8) 5_555 . -3_556 n
O5 La1 O5 125.529(22) 6_554 . -1_556 n
O5 La1 O5 65.689(8) 6_554 . -2_556 n
O5 La1 O5 46.054(11) 6_554 . -3_556 n
O5 La1 O5 115.444(20) -1_556 . -2_556 n
O5 La1 O5 105.165(15) -1_556 . -3_556 n
O5 La1 O5 111.738(19) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 136.466(22) -2_565 . 1_555 n
La2 La2 O1 136.472(22) -2_565 . 3_665 n
La2 La2 O1 136.505(22) -2_565 . 5_565 n
La2 La2 O2 44.947(24) -2_565 . 2_554 n
La2 La2 O2 44.935(24) -2_565 . 4_664 n
La2 La2 O2 44.932(24) -2_565 . 6_564 n
La2 La2 Sr2 89.976(16) -2_565 . 1_555 n
La2 La2 Sr2 0.0 -2_565 . -2_565 n
La2 La2 Sr2 179.972 -2_565 . -2_566 n
La2 La2 O1 43.520(22) -2_566 . 1_555 n
La2 La2 O1 43.511(22) -2_566 . 3_665 n
La2 La2 O1 43.526(22) -2_566 . 5_565 n
La2 La2 O2 135.082(24) -2_566 . 2_554 n
La2 La2 O2 135.042(24) -2_566 . 4_664 n
La2 La2 O2 135.062(24) -2_566 . 6_564 n
La2 La2 Sr2 89.976(16) -2_566 . 1_555 n
La2 La2 Sr2 179.972 -2_566 . -2_565 n
La2 La2 Sr2 0.0 -2_566 . -2_566 n
O1 La2 O1 73.211(35) 1_555 . 3_665 n
O1 La2 O1 73.217(35) 1_555 . 5_565 n
O1 La2 O2 125.051(28) 1_555 . 2_554 n
O1 La2 O2 93.704(24) 1_555 . 4_664 n
O1 La2 O2 154.229(31) 1_555 . 6_564 n
O1 La2 Sr2 54.673(11) 1_555 . 1_555 n
O1 La2 Sr2 136.466(22) 1_555 . -2_565 n
O1 La2 Sr2 43.519(22) 1_555 . -2_566 n
O1 La2 O1 73.222(35) 3_665 . 5_565 n
O1 La2 O2 154.271(31) 3_665 . 2_554 n
O1 La2 O2 125.036(28) 3_665 . 4_664 n
O1 La2 O2 93.724(24) 3_665 . 6_564 n
O1 La2 Sr2 87.990(25) 3_665 . 1_555 n
O1 La2 Sr2 136.480(22) 3_665 . -2_565 n
O1 La2 Sr2 43.519(22) 3_665 . -2_566 n
O1 La2 O2 93.736(24) 5_565 . 2_554 n
O1 La2 O2 154.243(31) 5_565 . 4_664 n
O1 La2 O2 125.075(28) 5_565 . 6_564 n
O1 La2 Sr2 127.801(19) 5_565 . 1_555 n
O1 La2 Sr2 136.497(22) 5_565 . -2_565 n
O1 La2 Sr2 43.519(22) 5_565 . -2_566 n
O2 La2 O2 75.42(4) 2_554 . 4_664 n
O2 La2 O2 75.43(4) 2_554 . 6_564 n
O2 La2 Sr2 117.027(19) 2_554 . 1_555 n
O2 La2 Sr2 44.938(24) 2_554 . -2_565 n
O2 La2 Sr2 135.074(24) 2_554 . -2_566 n
O2 La2 O2 75.42(4) 4_664 . 6_564 n
O2 La2 Sr2 45.907(26) 4_664 . 1_555 n
O2 La2 Sr2 44.938(24) 4_664 . -2_565 n
O2 La2 Sr2 135.044(24) 4_664 . -2_566 n
O2 La2 Sr2 103.894(25) 6_564 . 1_555 n
O2 La2 Sr2 44.938(24) 6_564 . -2_565 n
O2 La2 Sr2 135.068(24) 6_564 . -2_566 n
Sr2 La2 Sr2 89.996(12) 1_555 . -2_565 n
Sr2 La2 Sr2 89.996(12) 1_555 . -2_566 n
Sr2 La2 Sr2 180.0 -2_565 . -2_566 n
O1 SI O2 112.07(10) 1_555 . 1_555 n
O1 SI O3 110.79(6) 1_555 . 1_555 n
O1 SI O3 110.79(6) 1_555 . -4_556 n
O1 SI Sr1 130.44(7) 1_555 . 1_555 n
O1 SI Sr1 54.70(6) 1_555 . 3_555 n
O1 SI Sr2 136.59(5) 1_555 . 2_655 n
O1 SI Sr2 136.59(5) 1_555 . -1_665 n
O1 SI O5 88.20(6) 1_555 . 6_554 n
O1 SI O5 88.20(6) 1_555 . -3_556 n
O2 SI O3 108.40(6) 1_555 . 1_555 n
O2 SI O3 108.40(6) 1_555 . -4_556 n
O2 SI Sr1 117.49(7) 1_555 . 1_555 n
O2 SI Sr1 166.77(8) 1_555 . 3_555 n
O2 SI Sr2 48.58(4) 1_555 . 2_655 n
O2 SI Sr2 48.58(4) 1_555 . -1_665 n
O2 SI O5 140.12(5) 1_555 . 6_554 n
O2 SI O5 140.12(5) 1_555 . -3_556 n
O3 SI O3 106.17(9) 1_555 . -4_556 n
O3 SI Sr1 53.20(4) 1_555 . 1_555 n
O3 SI Sr1 79.03(5) 1_555 . 3_555 n
O3 SI Sr2 112.36(6) 1_555 . 2_655 n
O3 SI Sr2 60.66(4) 1_555 . -1_665 n
O3 SI O5 32.212(35) 1_555 . 6_554 n
O3 SI O5 94.49(7) 1_555 . -3_556 n
O3 SI Sr1 53.20(4) -4_556 . 1_555 n
O3 SI Sr1 79.03(5) -4_556 . 3_555 n
O3 SI Sr2 60.66(4) -4_556 . 2_655 n
O3 SI Sr2 112.36(6) -4_556 . -1_665 n
O3 SI O5 94.49(7) -4_556 . 6_554 n
O3 SI O5 32.212(35) -4_556 . -3_556 n
Sr1 SI Sr1 75.743(32) 1_555 . 3_555 n
Sr1 SI Sr2 81.250(25) 1_555 . 2_655 n
Sr1 SI Sr2 81.250(25) 1_555 . -1_665 n
Sr1 SI O5 53.117(32) 1_555 . 6_554 n
Sr1 SI O5 53.117(32) 1_555 . -3_556 n
Sr1 SI Sr2 139.644(26) 3_555 . 2_655 n
Sr1 SI Sr2 139.644(26) 3_555 . -1_665 n
Sr1 SI O5 46.877(31) 3_555 . 6_554 n
Sr1 SI O5 46.877(31) 3_555 . -3_556 n
Sr2 SI Sr2 65.97(4) 2_655 . -1_665 n
Sr2 SI O5 132.80(5) 2_655 . 6_554 n
Sr2 SI O5 92.864(30) 2_655 . -3_556 n
Sr2 SI O5 92.864(30) -1_665 . 6_554 n
Sr2 SI O5 132.80(5) -1_665 . -3_556 n
O5 SI O5 70.63(5) 6_554 . -3_556 n
La1 O1 La2 103.784(28) 3_555 . 1_555 n
La1 O1 La2 103.802(28) 3_555 . -2_566 n
La1 O1 SI 96.29(7) 3_555 . 1_555 n
La1 O1 Sr1 0.0 3_555 . 3_555 n
La1 O1 Sr2 103.789(28) 3_555 . 1_555 n
La1 O1 Sr2 103.789(28) 3_555 . -2_566 n
La2 O1 La2 92.95(4) 1_555 . -2_566 n
La2 O1 SI 128.036(33) 1_555 . 1_555 n
La2 O1 Sr1 103.784(28) 1_555 . 3_555 n
La2 O1 Sr2 0.0 1_555 . 1_555 n
La2 O1 Sr2 92.95(4) 1_555 . -2_566 n
La2 O1 SI 128.019(33) -2_566 . 1_555 n
La2 O1 Sr1 103.802(28) -2_566 . 3_555 n
La2 O1 Sr2 92.96(4) -2_566 . 1_555 n
La2 O1 Sr2 0.0 -2_566 . -2_566 n
SI O1 Sr1 96.29(7) 1_555 . 3_555 n
SI O1 Sr2 128.025(33) 1_555 . 1_555 n
SI O1 Sr2 128.025(33) 1_555 . -2_566 n
Sr1 O1 Sr2 103.789(28) 3_555 . 1_555 n
Sr1 O1 Sr2 103.789(28) 3_555 . -2_566 n
Sr2 O1 Sr2 92.96(4) 1_555 . -2_566 n
La1 O2 La2 115.366(30) 5_665 . 2_655 n
La1 O2 La2 115.359(30) 5_665 . -1_665 n
La1 O2 SI 124.36(7) 5_665 . 1_555 n
La1 O2 Sr1 0.0 5_665 . 5_665 n
La1 O2 Sr2 115.357(30) 5_665 . 2_655 n
La1 O2 Sr2 115.357(30) 5_665 . -1_665 n
La2 O2 La2 90.12(5) 2_655 . -1_665 n
La2 O2 SI 102.81(5) 2_655 . 1_555 n
La2 O2 Sr1 115.366(30) 2_655 . 5_665 n
La2 O2 Sr2 0.0 2_655 . 2_655 n
La2 O2 Sr2 90.13(5) 2_655 . -1_665 n
La2 O2 SI 102.83(5) -1_665 . 1_555 n
La2 O2 Sr1 115.359(30) -1_665 . 5_665 n
La2 O2 Sr2 90.12(5) -1_665 . 2_655 n
La2 O2 Sr2 0.0 -1_665 . -1_665 n
SI O2 Sr1 124.36(7) 1_555 . 5_665 n
SI O2 Sr2 102.83(5) 1_555 . 2_655 n
SI O2 Sr2 102.83(5) 1_555 . -1_665 n
Sr1 O2 Sr2 115.357(30) 5_665 . 2_655 n
Sr1 O2 Sr2 115.357(30) 5_665 . -1_665 n
Sr2 O2 Sr2 90.12(5) 2_655 . -1_665 n
La1 O3 La1 115.92(4) 1_555 . 2_554 n
La1 O3 SI 96.74(5) 1_555 . 1_555 n
La1 O3 Sr1 0.0 1_555 . 1_555 n
La1 O3 Sr1 115.92(4) 1_555 . 2_554 n
La1 O3 Sr2 101.617(27) 1_555 . -1_665 n
La1 O3 O5 78.67(5) 1_555 . 6_554 n
La1 O3 SI 142.59(6) 2_554 . 1_555 n
La1 O3 Sr1 115.92(4) 2_554 . 1_555 n
La1 O3 Sr1 0.0 2_554 . 2_554 n
La1 O3 Sr2 100.153(32) 2_554 . -1_665 n
La1 O3 O5 87.66(5) 2_554 . 6_554 n
SI O3 Sr1 96.74(5) 1_555 . 1_555 n
SI O3 Sr1 142.59(6) 1_555 . 2_554 n
SI O3 Sr2 89.92(6) 1_555 . -1_665 n
SI O3 O5 81.11(6) 1_555 . 6_554 n
Sr1 O3 Sr1 115.92(4) 1_555 . 2_554 n
Sr1 O3 Sr2 101.617(27) 1_555 . -1_665 n
Sr1 O3 O5 78.67(5) 1_555 . 6_554 n
Sr1 O3 Sr2 100.153(32) 2_554 . -1_665 n
Sr1 O3 O5 87.66(5) 2_554 . 6_554 n
Sr2 O3 O5 170.98(5) -1_665 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 Sr1 0.0 1_555 . 1_555 n
La1 O4 Sr1 120.0 1_555 . 3_555 n
La1 O4 Sr1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 3_555 . 1_555 n
La1 O4 Sr1 0.0 3_555 . 3_555 n
La1 O4 Sr1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 5_555 . 1_555 n
La1 O4 Sr1 120.0 5_555 . 3_555 n
La1 O4 Sr1 0.0 5_555 . 5_555 n
Sr1 O4 Sr1 120.0 1_555 . 3_555 n
Sr1 O4 Sr1 120.0 1_555 . 5_555 n
Sr1 O4 Sr1 120.0 3_555 . 5_555 n
La1 Sr1 La1 60.0 3_555 . 5_555 n
La1 Sr1 SI 53.180(28) 3_555 . 1_555 n
La1 Sr1 SI 111.077(27) 3_555 . 5_555 n
La1 Sr1 O1 140.087(30) 3_555 . 5_555 n
La1 Sr1 O2 120.05(4) 3_555 . 3_655 n
La1 Sr1 O3 57.263(24) 3_555 . 1_555 n
La1 Sr1 O3 109.443(24) 3_555 . 6_555 n
La1 Sr1 O3 109.443(24) 3_555 . -3_555 n
La1 Sr1 O3 57.263(24) 3_555 . -4_556 n
La1 Sr1 O4 30.0 3_555 . 1_555 n
La1 Sr1 Sr1 0.0 3_555 . 3_555 n
La1 Sr1 Sr1 60.0 3_555 . 5_555 n
La1 Sr1 Sr2 150.590(13) 3_555 . 1_545 n
La1 Sr1 Sr2 97.493(21) 3_555 . 2_655 n
La1 Sr1 Sr2 97.494(21) 3_555 . -1_665 n
La1 Sr1 Sr2 150.590(13) 3_555 . -2_556 n
La1 Sr1 O5 90.825(13) 3_555 . 4_554 n
La1 Sr1 O5 89.269(13) 3_555 . 5_555 n
La1 Sr1 O5 36.547(13) 3_555 . 6_554 n
La1 Sr1 O5 90.825(13) 3_555 . -1_556 n
La1 Sr1 O5 89.269(13) 3_555 . -2_556 n
La1 Sr1 O5 36.547(13) 3_555 . -3_556 n
La1 Sr1 SI 113.180(28) 5_555 . 1_555 n
La1 Sr1 SI 51.077(27) 5_555 . 5_555 n
La1 Sr1 O1 80.087(30) 5_555 . 5_555 n
La1 Sr1 O2 179.9557 5_555 . 3_655 n
La1 Sr1 O3 108.383(23) 5_555 . 1_555 n
La1 Sr1 O3 95.066(27) 5_555 . 6_555 n
La1 Sr1 O3 95.066(27) 5_555 . -3_555 n
La1 Sr1 O3 108.383(23) 5_555 . -4_556 n
La1 Sr1 O4 30.0 5_555 . 1_555 n
La1 Sr1 Sr1 60.0 5_555 . 3_555 n
La1 Sr1 Sr1 0.0 5_555 . 5_555 n
La1 Sr1 Sr2 104.331(21) 5_555 . 1_545 n
La1 Sr1 Sr2 147.307(14) 5_555 . 2_655 n
La1 Sr1 Sr2 147.307(14) 5_555 . -1_665 n
La1 Sr1 Sr2 104.331(21) 5_555 . -2_556 n
La1 Sr1 O5 38.445(14) 5_555 . 4_554 n
La1 Sr1 O5 90.785(13) 5_555 . 5_555 n
La1 Sr1 O5 89.264(13) 5_555 . 6_554 n
La1 Sr1 O5 38.445(14) 5_555 . -1_556 n
La1 Sr1 O5 90.785(13) 5_555 . -2_556 n
La1 Sr1 O5 89.264(13) 5_555 . -3_556 n
SI Sr1 SI 164.257(32) 1_555 . 5_555 n
SI Sr1 O1 166.73(4) 1_555 . 5_555 n
SI Sr1 O2 66.870(35) 1_555 . 3_655 n
SI Sr1 O3 30.055(16) 1_555 . 1_555 n
SI Sr1 O3 105.766(23) 1_555 . 6_555 n
SI Sr1 O3 105.766(23) 1_555 . -3_555 n
SI Sr1 O3 30.055(16) 1_555 . -4_556 n
SI Sr1 O4 83.180(28) 1_555 . 1_555 n
SI Sr1 Sr1 53.180(28) 1_555 . 3_555 n
SI Sr1 Sr1 113.180(28) 1_555 . 5_555 n
SI Sr1 Sr2 134.098(22) 1_555 . 1_545 n
SI Sr1 Sr2 50.246(21) 1_555 . 2_655 n
SI Sr1 Sr2 50.246(21) 1_555 . -1_665 n
SI Sr1 Sr2 134.098(22) 1_555 . -2_556 n
SI Sr1 O5 137.667(24) 1_555 . 4_554 n
SI Sr1 O5 88.498(14) 1_555 . 5_555 n
SI Sr1 O5 32.766(18) 1_555 . 6_554 n
SI Sr1 O5 137.667(24) 1_555 . -1_556 n
SI Sr1 O5 88.498(14) 1_555 . -2_556 n
SI Sr1 O5 32.766(18) 1_555 . -3_556 n
SI Sr1 O1 29.010(30) 5_555 . 5_555 n
SI Sr1 O2 128.87(4) 5_555 . 3_655 n
SI Sr1 O3 145.650(23) 5_555 . 1_555 n
SI Sr1 O3 78.236(23) 5_555 . 6_555 n
SI Sr1 O3 78.236(23) 5_555 . -3_555 n
SI Sr1 O3 145.650(23) 5_555 . -4_556 n
SI Sr1 O4 81.077(27) 5_555 . 1_555 n
SI Sr1 Sr1 111.077(27) 5_555 . 3_555 n
SI Sr1 Sr1 51.077(27) 5_555 . 5_555 n
SI Sr1 Sr2 58.944(20) 5_555 . 1_545 n
SI Sr1 Sr2 142.148(21) 5_555 . 2_655 n
SI Sr1 Sr2 142.148(21) 5_555 . -1_665 n
SI Sr1 Sr2 58.944(20) 5_555 . -2_556 n
SI Sr1 O5 31.041(15) 5_555 . 4_554 n
SI Sr1 O5 91.503(14) 5_555 . 5_555 n
SI Sr1 O5 135.061(26) 5_555 . 6_554 n
SI Sr1 O5 31.041(15) 5_555 . -1_556 n
SI Sr1 O5 91.503(14) 5_555 . -2_556 n
SI Sr1 O5 135.061(26) 5_555 . -3_556 n
O1 Sr1 O2 99.86(4) 5_555 . 3_655 n
O1 Sr1 O3 148.079(17) 5_555 . 1_555 n
O1 Sr1 O3 71.748(22) 5_555 . 6_555 n
O1 Sr1 O3 71.748(22) 5_555 . -3_555 n
O1 Sr1 O3 148.079(17) 5_555 . -4_556 n
O1 Sr1 O4 110.087(30) 5_555 . 1_555 n
O1 Sr1 Sr1 140.087(30) 5_555 . 3_555 n
O1 Sr1 Sr1 80.087(30) 5_555 . 5_555 n
O1 Sr1 Sr2 36.149(16) 5_555 . 1_545 n
O1 Sr1 Sr2 118.370(22) 5_555 . 2_655 n
O1 Sr1 Sr2 118.370(22) 5_555 . -1_665 n
O1 Sr1 Sr2 36.149(16) 5_555 . -2_556 n
O1 Sr1 O5 53.370(21) 5_555 . 4_554 n
O1 Sr1 O5 91.414(14) 5_555 . 5_555 n
O1 Sr1 O5 154.727(14) 5_555 . 6_554 n
O1 Sr1 O5 53.370(21) 5_555 . -1_556 n
O1 Sr1 O5 91.414(14) 5_555 . -2_556 n
O1 Sr1 O5 154.727(14) 5_555 . -3_556 n
O2 Sr1 O3 71.660(31) 3_655 . 1_555 n
O2 Sr1 O3 84.917(25) 3_655 . 6_555 n
O2 Sr1 O3 84.917(25) 3_655 . -3_555 n
O2 Sr1 O3 71.660(31) 3_655 . -4_556 n
O2 Sr1 O4 150.05(4) 3_655 . 1_555 n
O2 Sr1 Sr1 120.05(4) 3_655 . 3_555 n
O2 Sr1 Sr1 179.9557 3_655 . 5_555 n
O2 Sr1 Sr2 75.624(23) 3_655 . 1_545 n
O2 Sr1 Sr2 32.725(18) 3_655 . 2_655 n
O2 Sr1 Sr2 32.725(18) 3_655 . -1_665 n
O2 Sr1 Sr2 75.624(23) 3_655 . -2_556 n
O2 Sr1 O5 141.517(26) 3_655 . 4_554 n
O2 Sr1 O5 89.216(13) 3_655 . 5_555 n
O2 Sr1 O5 90.782(29) 3_655 . 6_554 n
O2 Sr1 O5 141.517(26) 3_655 . -1_556 n
O2 Sr1 O5 89.216(13) 3_655 . -2_556 n
O2 Sr1 O5 90.782(29) 3_655 . -3_556 n
O3 Sr1 O3 135.269(34) 1_555 . 6_555 n
O3 Sr1 O3 76.800(16) 1_555 . -3_555 n
O3 Sr1 O3 60.008(32) 1_555 . -4_556 n
O3 Sr1 O4 82.522(24) 1_555 . 1_555 n
O3 Sr1 Sr1 57.263(24) 1_555 . 3_555 n
O3 Sr1 Sr1 108.383(23) 1_555 . 5_555 n
O3 Sr1 Sr2 113.435(19) 1_555 . 1_545 n
O3 Sr1 Sr2 71.091(25) 1_555 . 2_655 n
O3 Sr1 Sr2 41.618(20) 1_555 . -1_665 n
O3 Sr1 Sr2 146.951(27) 1_555 . -2_556 n
O3 Sr1 O5 114.889(20) 1_555 . 4_554 n
O3 Sr1 O5 118.509(26) 1_555 . 5_555 n
O3 Sr1 O5 20.974(18) 1_555 . 6_554 n
O3 Sr1 O5 146.031(29) 1_555 . -1_556 n
O3 Sr1 O5 58.501(15) 1_555 . -2_556 n
O3 Sr1 O5 57.144(20) 1_555 . -3_556 n
O3 Sr1 O3 139.65(5) 6_555 . -3_555 n
O3 Sr1 O3 76.800(16) 6_555 . -4_556 n
O3 Sr1 O4 104.073(25) 6_555 . 1_555 n
O3 Sr1 Sr1 109.443(24) 6_555 . 3_555 n
O3 Sr1 Sr1 95.066(27) 6_555 . 5_555 n
O3 Sr1 Sr2 95.962(28) 6_555 . 1_545 n
O3 Sr1 Sr2 68.898(24) 6_555 . 2_655 n
O3 Sr1 Sr2 115.783(28) 6_555 . -1_665 n
O3 Sr1 Sr2 43.699(24) 6_555 . -2_556 n
O3 Sr1 O5 107.232(28) 6_555 . 4_554 n
O3 Sr1 O5 21.254(19) 6_555 . 5_555 n
O3 Sr1 O5 132.460(26) 6_555 . 6_554 n
O3 Sr1 O5 61.933(21) 6_555 . -1_556 n
O3 Sr1 O5 160.850(32) 6_555 . -2_556 n
O3 Sr1 O5 86.604(20) 6_555 . -3_556 n
O3 Sr1 O3 135.268(34) -3_555 . -4_556 n
O3 Sr1 O4 104.073(25) -3_555 . 1_555 n
O3 Sr1 Sr1 109.443(24) -3_555 . 3_555 n
O3 Sr1 Sr1 95.066(27) -3_555 . 5_555 n
O3 Sr1 Sr2 43.699(24) -3_555 . 1_545 n
O3 Sr1 Sr2 115.783(28) -3_555 . 2_655 n
O3 Sr1 Sr2 68.898(24) -3_555 . -1_665 n
O3 Sr1 Sr2 95.962(28) -3_555 . -2_556 n
O3 Sr1 O5 61.933(21) -3_555 . 4_554 n
O3 Sr1 O5 160.850(32) -3_555 . 5_555 n
O3 Sr1 O5 86.604(20) -3_555 . 6_554 n
O3 Sr1 O5 107.232(28) -3_555 . -1_556 n
O3 Sr1 O5 21.254(19) -3_555 . -2_556 n
O3 Sr1 O5 132.460(26) -3_555 . -3_556 n
O3 Sr1 O4 82.522(24) -4_556 . 1_555 n
O3 Sr1 Sr1 57.263(24) -4_556 . 3_555 n
O3 Sr1 Sr1 108.383(23) -4_556 . 5_555 n
O3 Sr1 Sr2 146.951(27) -4_556 . 1_545 n
O3 Sr1 Sr2 41.618(20) -4_556 . 2_655 n
O3 Sr1 Sr2 71.091(25) -4_556 . -1_665 n
O3 Sr1 Sr2 113.435(19) -4_556 . -2_556 n
O3 Sr1 O5 146.031(29) -4_556 . 4_554 n
O3 Sr1 O5 58.501(15) -4_556 . 5_555 n
O3 Sr1 O5 57.144(20) -4_556 . 6_554 n
O3 Sr1 O5 114.889(20) -4_556 . -1_556 n
O3 Sr1 O5 118.509(26) -4_556 . -2_556 n
O3 Sr1 O5 20.974(18) -4_556 . -3_556 n
O4 Sr1 Sr1 30.0 1_555 . 3_555 n
O4 Sr1 Sr1 30.0 1_555 . 5_555 n
O4 Sr1 Sr2 130.230(19) 1_555 . 1_545 n
O4 Sr1 Sr2 124.137(19) 1_555 . 2_655 n
O4 Sr1 Sr2 124.137(19) 1_555 . -1_665 n
O4 Sr1 Sr2 130.230(19) 1_555 . -2_556 n
O4 Sr1 O5 63.649(14) 1_555 . 4_554 n
O4 Sr1 O5 90.031(12) 1_555 . 5_555 n
O4 Sr1 O5 61.885(14) 1_555 . 6_554 n
O4 Sr1 O5 63.649(14) 1_555 . -1_556 n
O4 Sr1 O5 90.031(12) 1_555 . -2_556 n
O4 Sr1 O5 61.885(14) 1_555 . -3_556 n
Sr1 Sr1 Sr1 60.0 3_555 . 5_555 n
Sr1 Sr1 Sr2 150.590(13) 3_555 . 1_545 n
Sr1 Sr1 Sr2 97.493(21) 3_555 . 2_655 n
Sr1 Sr1 Sr2 97.494(21) 3_555 . -1_665 n
Sr1 Sr1 Sr2 150.590(13) 3_555 . -2_556 n
Sr1 Sr1 O5 90.825(13) 3_555 . 4_554 n
Sr1 Sr1 O5 89.269(13) 3_555 . 5_555 n
Sr1 Sr1 O5 36.547(13) 3_555 . 6_554 n
Sr1 Sr1 O5 90.825(13) 3_555 . -1_556 n
Sr1 Sr1 O5 89.269(13) 3_555 . -2_556 n
Sr1 Sr1 O5 36.547(13) 3_555 . -3_556 n
Sr1 Sr1 Sr2 104.331(21) 5_555 . 1_545 n
Sr1 Sr1 Sr2 147.307(14) 5_555 . 2_655 n
Sr1 Sr1 Sr2 147.307(14) 5_555 . -1_665 n
Sr1 Sr1 Sr2 104.331(21) 5_555 . -2_556 n
Sr1 Sr1 O5 38.445(14) 5_555 . 4_554 n
Sr1 Sr1 O5 90.785(13) 5_555 . 5_555 n
Sr1 Sr1 O5 89.264(13) 5_555 . 6_554 n
Sr1 Sr1 O5 38.445(14) 5_555 . -1_556 n
Sr1 Sr1 O5 90.785(13) 5_555 . -2_556 n
Sr1 Sr1 O5 89.264(13) 5_555 . -3_556 n
Sr2 Sr1 Sr2 105.519(12) 1_545 . 2_655 n
Sr2 Sr1 Sr2 83.945(8) 1_545 . -1_665 n
Sr2 Sr1 Sr2 52.265(24) 1_545 . -2_556 n
Sr2 Sr1 O5 67.008(12) 1_545 . 4_554 n
Sr2 Sr1 O5 117.158(21) 1_545 . 5_555 n
Sr2 Sr1 O5 128.685(12) 1_545 . 6_554 n
Sr2 Sr1 O5 88.234(18) 1_545 . -1_556 n
Sr2 Sr1 O5 64.904(14) 1_545 . -2_556 n
Sr2 Sr1 O5 165.838(21) 1_545 . -3_556 n
Sr2 Sr1 Sr2 50.109(24) 2_655 . -1_665 n
Sr2 Sr1 Sr2 83.945(8) 2_655 . -2_556 n
Sr2 Sr1 O5 171.599(21) 2_655 . 4_554 n
Sr2 Sr1 O5 63.739(14) 2_655 . 5_555 n
Sr2 Sr1 O5 82.410(17) 2_655 . 6_554 n
Sr2 Sr1 O5 130.042(12) 2_655 . -1_556 n
Sr2 Sr1 O5 113.841(21) 2_655 . -2_556 n
Sr2 Sr1 O5 62.394(11) 2_655 . -3_556 n
Sr2 Sr1 Sr2 105.519(12) -1_665 . -2_556 n
Sr2 Sr1 O5 130.042(12) -1_665 . 4_554 n
Sr2 Sr1 O5 113.841(21) -1_665 . 5_555 n
Sr2 Sr1 O5 62.394(11) -1_665 . 6_554 n
Sr2 Sr1 O5 171.599(21) -1_665 . -1_556 n
Sr2 Sr1 O5 63.739(14) -1_665 . -2_556 n
Sr2 Sr1 O5 82.410(17) -1_665 . -3_556 n
Sr2 Sr1 O5 88.234(18) -2_556 . 4_554 n
Sr2 Sr1 O5 64.904(14) -2_556 . 5_555 n
Sr2 Sr1 O5 165.838(21) -2_556 . 6_554 n
Sr2 Sr1 O5 67.008(12) -2_556 . -1_556 n
Sr2 Sr1 O5 117.158(21) -2_556 . -2_556 n
Sr2 Sr1 O5 128.685(12) -2_556 . -3_556 n
O5 Sr1 O5 115.444(20) 4_554 . 5_555 n
O5 Sr1 O5 105.165(15) 4_554 . 6_554 n
O5 Sr1 O5 48.212(12) 4_554 . -1_556 n
O5 Sr1 O5 67.236(8) 4_554 . -2_556 n
O5 Sr1 O5 125.529(22) 4_554 . -3_556 n
O5 Sr1 O5 111.738(19) 5_555 . 6_554 n
O5 Sr1 O5 67.236(8) 5_555 . -1_556 n
O5 Sr1 O5 176.966(29) 5_555 . -2_556 n
O5 Sr1 O5 65.689(8) 5_555 . -3_556 n
O5 Sr1 O5 125.529(22) 6_554 . -1_556 n
O5 Sr1 O5 65.689(8) 6_554 . -2_556 n
O5 Sr1 O5 46.054(11) 6_554 . -3_556 n
O5 Sr1 O5 115.444(20) -1_556 . -2_556 n
O5 Sr1 O5 105.165(15) -1_556 . -3_556 n
O5 Sr1 O5 111.738(19) -2_556 . -3_556 n
La2 Sr2 La2 90.0091 1_555 . -2_565 n
La2 Sr2 La2 90.009 1_555 . -2_566 n
La2 Sr2 SI 84.689(19) 1_555 . 2_554 n
La2 Sr2 SI 140.148(27) 1_555 . 4_664 n
La2 Sr2 SI 47.517(23) 1_555 . 6_564 n
La2 Sr2 O1 125.314(22) 1_555 . 1_555 n
La2 Sr2 O1 91.978(28) 1_555 . 3_665 n
La2 Sr2 O1 52.191(25) 1_555 . 5_565 n
La2 Sr2 O2 62.941(23) 1_555 . 2_554 n
La2 Sr2 O2 134.057(27) 1_555 . 4_664 n
La2 Sr2 O2 76.097(18) 1_555 . 6_564 n
La2 Sr2 O3 135.460(17) 1_555 . -1_665 n
La2 Sr2 O3 19.274(17) 1_555 . -3_565 n
La2 Sr2 O3 103.406(16) 1_555 . -5_555 n
La2 Sr2 Sr1 30.716(13) 1_555 . 1_565 n
La2 Sr2 Sr1 133.113(7) 1_555 . 2_554 n
La2 Sr2 Sr1 101.913(8) 1_555 . 3_555 n
La2 Sr2 Sr1 99.969(8) 1_555 . 4_664 n
La2 Sr2 Sr1 130.8099 1_555 . 5_665 n
La2 Sr2 Sr1 31.075(14) 1_555 . 6_564 n
La2 Sr2 Sr2 90.000(6) 1_555 . -2_565 n
La2 Sr2 Sr2 90.000(6) 1_555 . -2_566 n
La2 Sr2 La2 180.0 -2_565 . -2_566 n
La2 Sr2 SI 57.023(18) -2_565 . 2_554 n
La2 Sr2 SI 57.008(18) -2_565 . 4_664 n
La2 Sr2 SI 57.014(18) -2_565 . 6_564 n
La2 Sr2 O1 136.481(22) -2_565 . 1_555 n
La2 Sr2 O1 136.473(22) -2_565 . 3_665 n
La2 Sr2 O1 136.489(22) -2_565 . 5_565 n
La2 Sr2 O2 44.947(24) -2_565 . 2_554 n
La2 Sr2 O2 44.935(24) -2_565 . 4_664 n
La2 Sr2 O2 44.932(24) -2_565 . 6_564 n
La2 Sr2 O3 79.977(21) -2_565 . -1_665 n
La2 Sr2 O3 79.988(21) -2_565 . -3_565 n
La2 Sr2 O3 79.992(21) -2_565 . -5_555 n
La2 Sr2 Sr1 116.135(12) -2_565 . 1_565 n
La2 Sr2 Sr1 64.947(12) -2_565 . 2_554 n
La2 Sr2 Sr1 116.139(12) -2_565 . 3_555 n
La2 Sr2 Sr1 64.937(12) -2_565 . 4_664 n
La2 Sr2 Sr1 116.124(12) -2_565 . 5_665 n
La2 Sr2 Sr1 64.952(12) -2_565 . 6_564 n
La2 Sr2 Sr2 0.0 -2_565 . -2_565 n
La2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La2 Sr2 SI 122.993(18) -2_566 . 2_554 n
La2 Sr2 SI 122.978(18) -2_566 . 4_664 n
La2 Sr2 SI 122.984(18) -2_566 . 6_564 n
La2 Sr2 O1 43.519(22) -2_566 . 1_555 n
La2 Sr2 O1 43.511(22) -2_566 . 3_665 n
La2 Sr2 O1 43.526(22) -2_566 . 5_565 n
La2 Sr2 O2 135.071(24) -2_566 . 2_554 n
La2 Sr2 O2 135.059(24) -2_566 . 4_664 n
La2 Sr2 O2 135.056(24) -2_566 . 6_564 n
La2 Sr2 O3 100.006(21) -2_566 . -1_665 n
La2 Sr2 O3 100.017(21) -2_566 . -3_565 n
La2 Sr2 O3 100.021(21) -2_566 . -5_555 n
La2 Sr2 Sr1 63.870(12) -2_566 . 1_565 n
La2 Sr2 Sr1 115.056(12) -2_566 . 2_554 n
La2 Sr2 Sr1 63.874(12) -2_566 . 3_555 n
La2 Sr2 Sr1 115.046(12) -2_566 . 4_664 n
La2 Sr2 Sr1 63.859(12) -2_566 . 5_665 n
La2 Sr2 Sr1 115.061(12) -2_566 . 6_564 n
La2 Sr2 Sr2 180.0 -2_566 . -2_565 n
La2 Sr2 Sr2 0.0 -2_566 . -2_566 n
SI Sr2 SI 93.177(24) 2_554 . 4_664 n
SI Sr2 SI 93.177(24) 2_554 . 6_564 n
SI Sr2 O1 97.859(29) 2_554 . 1_555 n
SI Sr2 O1 166.247(34) 2_554 . 3_665 n
SI Sr2 O1 94.375(23) 2_554 . 5_565 n
SI Sr2 O2 28.592(27) 2_554 . 2_554 n
SI Sr2 O2 64.908(29) 2_554 . 4_664 n
SI Sr2 O2 98.39(4) 2_554 . 6_564 n
SI Sr2 O3 122.544(32) 2_554 . -1_665 n
SI Sr2 O3 92.810(28) 2_554 . -3_565 n
SI Sr2 O3 29.427(21) 2_554 . -5_555 n
SI Sr2 Sr1 112.043(21) 2_554 . 1_565 n
SI Sr2 Sr1 48.504(23) 2_554 . 2_554 n
SI Sr2 Sr1 61.998(15) 2_554 . 3_555 n
SI Sr2 Sr1 121.792(27) 2_554 . 4_664 n
SI Sr2 Sr1 144.445(23) 2_554 . 5_665 n
SI Sr2 Sr1 56.227(22) 2_554 . 6_564 n
SI Sr2 Sr2 57.015(18) 2_554 . -2_565 n
SI Sr2 Sr2 122.985(18) 2_554 . -2_566 n
SI Sr2 SI 93.177(24) 4_664 . 6_564 n
SI Sr2 O1 94.374(23) 4_664 . 1_555 n
SI Sr2 O1 97.859(29) 4_664 . 3_665 n
SI Sr2 O1 166.247(34) 4_664 . 5_565 n
SI Sr2 O2 98.39(4) 4_664 . 2_554 n
SI Sr2 O2 28.592(27) 4_664 . 4_664 n
SI Sr2 O2 64.908(29) 4_664 . 6_564 n
SI Sr2 O3 29.427(21) 4_664 . -1_665 n
SI Sr2 O3 122.544(32) 4_664 . -3_565 n
SI Sr2 O3 92.810(28) 4_664 . -5_555 n
SI Sr2 Sr1 144.445(23) 4_664 . 1_565 n
SI Sr2 Sr1 56.226(22) 4_664 . 2_554 n
SI Sr2 Sr1 112.043(21) 4_664 . 3_555 n
SI Sr2 Sr1 48.504(23) 4_664 . 4_664 n
SI Sr2 Sr1 61.998(15) 4_664 . 5_665 n
SI Sr2 Sr1 121.792(27) 4_664 . 6_564 n
SI Sr2 Sr2 57.015(18) 4_664 . -2_565 n
SI Sr2 Sr2 122.984(18) 4_664 . -2_566 n
SI Sr2 O1 166.247(34) 6_564 . 1_555 n
SI Sr2 O1 94.375(23) 6_564 . 3_665 n
SI Sr2 O1 97.859(29) 6_564 . 5_565 n
SI Sr2 O2 64.908(29) 6_564 . 2_554 n
SI Sr2 O2 98.39(4) 6_564 . 4_664 n
SI Sr2 O2 28.593(27) 6_564 . 6_564 n
SI Sr2 O3 92.810(28) 6_564 . -1_665 n
SI Sr2 O3 29.427(21) 6_564 . -3_565 n
SI Sr2 O3 122.544(32) 6_564 . -5_555 n
SI Sr2 Sr1 61.998(15) 6_564 . 1_565 n
SI Sr2 Sr1 121.792(27) 6_564 . 2_554 n
SI Sr2 Sr1 144.445(23) 6_564 . 3_555 n
SI Sr2 Sr1 56.226(22) 6_564 . 4_664 n
SI Sr2 Sr1 112.043(21) 6_564 . 5_665 n
SI Sr2 Sr1 48.504(23) 6_564 . 6_564 n
SI Sr2 Sr2 57.015(18) 6_564 . -2_565 n
SI Sr2 Sr2 122.985(18) 6_564 . -2_566 n
O1 Sr2 O1 73.216(35) 1_555 . 3_665 n
O1 Sr2 O1 73.216(35) 1_555 . 5_565 n
O1 Sr2 O2 125.054(28) 1_555 . 2_554 n
O1 Sr2 O2 93.721(24) 1_555 . 4_664 n
O1 Sr2 O2 154.248(31) 1_555 . 6_564 n
O1 Sr2 O3 88.166(28) 1_555 . -1_665 n
O1 Sr2 O3 140.916(34) 1_555 . -3_565 n
O1 Sr2 O3 68.535(29) 1_555 . -5_555 n
O1 Sr2 Sr1 105.924(30) 1_555 . 1_565 n
O1 Sr2 Sr1 71.912(19) 1_555 . 2_554 n
O1 Sr2 Sr1 40.062(26) 1_555 . 3_555 n
O1 Sr2 Sr1 122.658(25) 1_555 . 4_664 n
O1 Sr2 Sr1 62.148(28) 1_555 . 5_665 n
O1 Sr2 Sr1 133.797(25) 1_555 . 6_564 n
O1 Sr2 Sr2 136.481(22) 1_555 . -2_565 n
O1 Sr2 Sr2 43.519(22) 1_555 . -2_566 n
O1 Sr2 O1 73.217(35) 3_665 . 5_565 n
O1 Sr2 O2 154.248(31) 3_665 . 2_554 n
O1 Sr2 O2 125.054(28) 3_665 . 4_664 n
O1 Sr2 O2 93.721(24) 3_665 . 6_564 n
O1 Sr2 O3 68.535(29) 3_665 . -1_665 n
O1 Sr2 O3 88.167(28) 3_665 . -3_565 n
O1 Sr2 O3 140.916(34) 3_665 . -5_555 n
O1 Sr2 Sr1 62.148(28) 3_665 . 1_565 n
O1 Sr2 Sr1 133.796(25) 3_665 . 2_554 n
O1 Sr2 Sr1 105.924(30) 3_665 . 3_555 n
O1 Sr2 Sr1 71.912(19) 3_665 . 4_664 n
O1 Sr2 Sr1 40.062(26) 3_665 . 5_665 n
O1 Sr2 Sr1 122.658(25) 3_665 . 6_564 n
O1 Sr2 Sr2 136.481(22) 3_665 . -2_565 n
O1 Sr2 Sr2 43.519(22) 3_665 . -2_566 n
O1 Sr2 O2 93.721(24) 5_565 . 2_554 n
O1 Sr2 O2 154.248(31) 5_565 . 4_664 n
O1 Sr2 O2 125.054(28) 5_565 . 6_564 n
O1 Sr2 O3 140.916(34) 5_565 . -1_665 n
O1 Sr2 O3 68.536(29) 5_565 . -3_565 n
O1 Sr2 O3 88.167(28) 5_565 . -5_555 n
O1 Sr2 Sr1 40.062(26) 5_565 . 1_565 n
O1 Sr2 Sr1 122.658(25) 5_565 . 2_554 n
O1 Sr2 Sr1 62.148(28) 5_565 . 3_555 n
O1 Sr2 Sr1 133.797(25) 5_565 . 4_664 n
O1 Sr2 Sr1 105.924(30) 5_565 . 5_665 n
O1 Sr2 Sr1 71.912(19) 5_565 . 6_564 n
O1 Sr2 Sr2 136.481(22) 5_565 . -2_565 n
O1 Sr2 Sr2 43.519(22) 5_565 . -2_566 n
O2 Sr2 O2 75.43(4) 2_554 . 4_664 n
O2 Sr2 O2 75.43(4) 2_554 . 6_564 n
O2 Sr2 O3 124.63(4) 2_554 . -1_665 n
O2 Sr2 O3 66.235(27) 2_554 . -3_565 n
O2 Sr2 O3 57.681(23) 2_554 . -5_555 n
O2 Sr2 Sr1 93.450(22) 2_554 . 1_565 n
O2 Sr2 Sr1 71.949(27) 2_554 . 2_554 n
O2 Sr2 Sr1 86.187(19) 2_554 . 3_555 n
O2 Sr2 Sr1 105.032(30) 2_554 . 4_664 n
O2 Sr2 Sr1 160.337(34) 2_554 . 5_665 n
O2 Sr2 Sr1 31.918(23) 2_554 . 6_564 n
O2 Sr2 Sr2 44.938(24) 2_554 . -2_565 n
O2 Sr2 Sr2 135.062(24) 2_554 . -2_566 n
O2 Sr2 O2 75.43(4) 4_664 . 6_564 n
O2 Sr2 O3 57.681(23) 4_664 . -1_665 n
O2 Sr2 O3 124.63(4) 4_664 . -3_565 n
O2 Sr2 O3 66.235(27) 4_664 . -5_555 n
O2 Sr2 Sr1 160.337(34) 4_664 . 1_565 n
O2 Sr2 Sr1 31.918(23) 4_664 . 2_554 n
O2 Sr2 Sr1 93.449(22) 4_664 . 3_555 n
O2 Sr2 Sr1 71.949(27) 4_664 . 4_664 n
O2 Sr2 Sr1 86.186(19) 4_664 . 5_665 n
O2 Sr2 Sr1 105.032(30) 4_664 . 6_564 n
O2 Sr2 Sr2 44.938(24) 4_664 . -2_565 n
O2 Sr2 Sr2 135.062(24) 4_664 . -2_566 n
O2 Sr2 O3 66.235(27) 6_564 . -1_665 n
O2 Sr2 O3 57.681(23) 6_564 . -3_565 n
O2 Sr2 O3 124.63(4) 6_564 . -5_555 n
O2 Sr2 Sr1 86.187(19) 6_564 . 1_565 n
O2 Sr2 Sr1 105.032(30) 6_564 . 2_554 n
O2 Sr2 Sr1 160.337(34) 6_564 . 3_555 n
O2 Sr2 Sr1 31.918(23) 6_564 . 4_664 n
O2 Sr2 Sr1 93.449(22) 6_564 . 5_665 n
O2 Sr2 Sr1 71.949(27) 6_564 . 6_564 n
O2 Sr2 Sr2 44.938(24) 6_564 . -2_565 n
O2 Sr2 Sr2 135.062(24) 6_564 . -2_566 n
O3 Sr2 O3 117.042(12) -1_665 . -3_565 n
O3 Sr2 O3 117.042(12) -1_665 . -5_555 n
O3 Sr2 Sr1 120.928(20) -1_665 . 1_565 n
O3 Sr2 Sr1 80.960(19) -1_665 . 2_554 n
O3 Sr2 Sr1 121.554(20) -1_665 . 3_555 n
O3 Sr2 Sr1 36.765(18) -1_665 . 4_664 n
O3 Sr2 Sr1 36.148(14) -1_665 . 5_665 n
O3 Sr2 Sr1 137.501(27) -1_665 . 6_564 n
O3 Sr2 Sr2 79.985(21) -1_665 . -2_565 n
O3 Sr2 Sr2 100.014(21) -1_665 . -2_566 n
O3 Sr2 O3 117.042(12) -3_565 . -5_555 n
O3 Sr2 Sr1 36.149(14) -3_565 . 1_565 n
O3 Sr2 Sr1 137.501(27) -3_565 . 2_554 n
O3 Sr2 Sr1 120.928(20) -3_565 . 3_555 n
O3 Sr2 Sr1 80.960(19) -3_565 . 4_664 n
O3 Sr2 Sr1 121.554(20) -3_565 . 5_665 n
O3 Sr2 Sr1 36.765(18) -3_565 . 6_564 n
O3 Sr2 Sr2 79.986(21) -3_565 . -2_565 n
O3 Sr2 Sr2 100.015(21) -3_565 . -2_566 n
O3 Sr2 Sr1 121.554(20) -5_555 . 1_565 n
O3 Sr2 Sr1 36.765(18) -5_555 . 2_554 n
O3 Sr2 Sr1 36.149(14) -5_555 . 3_555 n
O3 Sr2 Sr1 137.501(27) -5_555 . 4_664 n
O3 Sr2 Sr1 120.928(20) -5_555 . 5_665 n
O3 Sr2 Sr1 80.960(19) -5_555 . 6_564 n
O3 Sr2 Sr2 79.986(21) -5_555 . -2_565 n
O3 Sr2 Sr2 100.015(21) -5_555 . -2_566 n
Sr1 Sr2 Sr1 158.106(12) 1_565 . 2_554 n
Sr1 Sr2 Sr1 102.064(15) 1_565 . 3_555 n
Sr1 Sr2 Sr1 96.055(8) 1_565 . 4_664 n
Sr1 Sr2 Sr1 102.064(15) 1_565 . 5_665 n
Sr1 Sr2 Sr1 61.719(10) 1_565 . 6_564 n
Sr1 Sr2 Sr2 116.133(12) 1_565 . -2_565 n
Sr1 Sr2 Sr2 63.868(12) 1_565 . -2_566 n
Sr1 Sr2 Sr1 61.719(10) 2_554 . 3_555 n
Sr1 Sr2 Sr1 103.356(14) 2_554 . 4_664 n
Sr1 Sr2 Sr1 96.054(8) 2_554 . 5_665 n
Sr1 Sr2 Sr1 103.356(14) 2_554 . 6_564 n
Sr1 Sr2 Sr2 64.946(12) 2_554 . -2_565 n
Sr1 Sr2 Sr2 115.054(12) 2_554 . -2_566 n
Sr1 Sr2 Sr1 158.106(12) 3_555 . 4_664 n
Sr1 Sr2 Sr1 102.064(15) 3_555 . 5_665 n
Sr1 Sr2 Sr1 96.055(8) 3_555 . 6_564 n
Sr1 Sr2 Sr2 116.132(12) 3_555 . -2_565 n
Sr1 Sr2 Sr2 63.868(12) 3_555 . -2_566 n
Sr1 Sr2 Sr1 61.719(10) 4_664 . 5_665 n
Sr1 Sr2 Sr1 103.356(14) 4_664 . 6_564 n
Sr1 Sr2 Sr2 64.946(12) 4_664 . -2_565 n
Sr1 Sr2 Sr2 115.054(12) 4_664 . -2_566 n
Sr1 Sr2 Sr1 158.106(12) 5_665 . 6_564 n
Sr1 Sr2 Sr2 116.132(12) 5_665 . -2_565 n
Sr1 Sr2 Sr2 63.867(12) 5_665 . -2_566 n
Sr1 Sr2 Sr2 64.946(12) 6_564 . -2_565 n
Sr1 Sr2 Sr2 115.054(12) 6_564 . -2_566 n
Sr2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La1 O5 La1 111.686(18) 2_555 . 3_555 n
La1 O5 La1 105.008(21) 2_555 . 4_555 n
La1 O5 SI 94.12(4) 2_555 . 2_555 n
La1 O5 O3 80.36(5) 2_555 . 2_555 n
La1 O5 Sr1 0.0 2_555 . 2_555 n
La1 O5 Sr1 111.686(18) 2_555 . 3_555 n
La1 O5 Sr1 105.008(21) 2_555 . 4_555 n
La1 O5 La1 115.389(18) 3_555 . 4_555 n
La1 O5 SI 125.180(27) 3_555 . 2_555 n
La1 O5 O3 71.08(4) 3_555 . 2_555 n
La1 O5 Sr1 111.686(18) 3_555 . 2_555 n
La1 O5 Sr1 0.0 3_555 . 3_555 n
La1 O5 Sr1 115.389(18) 3_555 . 4_555 n
La1 O5 SI 102.08(4) 4_555 . 2_555 n
La1 O5 O3 168.14(5) 4_555 . 2_555 n
La1 O5 Sr1 105.008(21) 4_555 . 2_555 n
La1 O5 Sr1 115.389(18) 4_555 . 3_555 n
La1 O5 Sr1 0.0 4_555 . 4_555 n
SI O5 O3 66.67(6) 2_555 . 2_555 n
SI O5 Sr1 94.12(4) 2_555 . 2_555 n
SI O5 Sr1 125.180(27) 2_555 . 3_555 n
SI O5 Sr1 102.08(4) 2_555 . 4_555 n
O3 O5 Sr1 80.36(5) 2_555 . 2_555 n
O3 O5 Sr1 71.08(4) 2_555 . 3_555 n
O3 O5 Sr1 168.14(5) 2_555 . 4_555 n
Sr1 O5 Sr1 111.686(18) 2_555 . 3_555 n
Sr1 O5 Sr1 105.008(21) 2_555 . 4_555 n
Sr1 O5 Sr1 115.389(18) 3_555 . 4_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.0252(10) . 3_555 n
La1 La1 4.0252(10) . 5_555 n
La1 La2 4.1185(7) . 1_545 n
La1 La2 4.1191(7) . -2_556 n
La1 SI 3.2311(13) . 1_555 n
La1 SI 3.3247(15) . 5_555 n
La1 O1 2.7297(13) . 5_555 n
La1 O2 2.4946(12) . 3_655 n
La1 O3 2.6053(10) . 1_555 n
La1 O3 2.4684(7) . 6_555 n
La1 O3 2.4684(7) . -3_555 n
La1 O3 2.6053(10) . -4_556 n
La1 O4 2.3240(5) . 1_555 n
La1 Sr1 4.30157(30) . 2_554 n
La1 Sr1 4.30157(30) . 2_555 n
La1 Sr1 4.0252(10) . 3_555 n
La1 Sr1 4.0252(10) . 5_555 n
La1 Sr1 4.30157(30) . 6_554 n
La1 Sr1 4.30157(30) . 6_555 n
La1 Sr2 4.1190(7) . 1_545 n
La1 Sr2 4.2637(7) . 2_655 n
La1 Sr2 4.2637(7) . -1_665 n
La1 Sr2 4.1190(7) . -2_556 n
La1 O5 2.4816(6) . 4_554 n
La1 O5 2.607160(30) . 5_555 n
La1 O5 2.5911(6) . 6_554 n
La1 O5 2.4816(6) . -1_556 n
La1 O5 2.607160(30) . -2_556 n
La1 O5 2.5911(6) . -3_556 n
La2 La1 4.1185(7) . 1_565 n
La2 La1 4.1191(7) . 3_555 n
La2 La1 4.1194(7) . 5_665 n
La2 La2 3.6111(18) . -2_565 n
La2 La2 3.6284(18) . -2_566 n
La2 SI 3.3165(12) . 2_554 n
La2 SI 3.3169(12) . 4_664 n
La2 SI 3.3161(12) . 6_564 n
La2 O1 2.5022(10) . 1_555 n
La2 O1 2.5019(10) . 3_665 n
La2 O1 2.5015(10) . 5_565 n
La2 O2 2.5504(10) . 2_554 n
La2 O2 2.5511(10) . 4_664 n
La2 O2 2.5506(10) . 6_564 n
La2 O3 2.8914(9) . -1_665 n
La2 O3 2.8904(9) . -3_565 n
La2 O3 2.8911(9) . -5_555 n
La2 Sr1 4.1185(7) . 1_565 n
La2 Sr1 4.2641(7) . 2_554 n
La2 Sr1 4.1191(7) . 3_555 n
La2 Sr1 4.2638(7) . 4_664 n
La2 Sr1 4.1194(7) . 5_665 n
La2 Sr1 4.2632(7) . 6_564 n
La2 Sr2 0.00056 . 1_555 n
La2 Sr2 3.6111(18) . -2_565 n
La2 Sr2 3.6284(18) . -2_566 n
SI La1 3.2311(13) . 1_555 n
SI La1 3.3247(15) . 3_555 n
SI La2 3.3161(12) . 2_655 n
SI La2 3.3169(12) . -1_665 n
SI O1 1.6221(16) . 1_555 n
SI O2 1.6278(16) . 1_555 n
SI O3 1.6295(10) . 1_555 n
SI O3 1.6295(10) . -4_556 n
SI Sr1 3.2311(13) . 1_555 n
SI Sr1 3.3247(15) . 3_555 n
SI Sr1 3.6683(14) . 5_665 n
SI Sr2 3.7270(11) . 1_555 n
SI Sr2 3.3165(12) . 2_655 n
SI Sr2 3.3165(12) . -1_665 n
SI Sr2 3.7270(11) . -2_566 n
SI O5 1.7532(10) . 6_554 n
SI O5 1.7532(10) . -3_556 n
O1 La1 2.7297(13) . 3_555 n
O1 La2 2.5022(10) . 1_555 n
O1 La2 2.5019(10) . -2_566 n
O1 SI 1.6221(16) . 1_555 n
O1 Sr1 2.7297(13) . 3_555 n
O1 Sr2 2.5019(10) . 1_555 n
O1 Sr2 2.5019(10) . -2_566 n
O2 La1 2.4946(12) . 5_665 n
O2 La2 2.5506(10) . 2_655 n
O2 La2 2.5511(10) . -1_665 n
O2 SI 1.6278(16) . 1_555 n
O2 Sr1 2.4946(12) . 5_665 n
O2 Sr2 2.5507(10) . 2_655 n
O2 Sr2 2.5507(10) . -1_665 n
O3 La1 2.6053(10) . 1_555 n
O3 La1 2.4684(7) . 2_554 n
O3 La2 2.8914(9) . -1_665 n
O3 SI 1.6295(10) . 1_555 n
O3 Sr1 2.6053(10) . 1_555 n
O3 Sr1 2.4684(7) . 2_554 n
O3 Sr1 3.4128(10) . 3_555 n
O3 Sr2 2.8910(9) . -1_665 n
O3 O5 0.9459(8) . 6_554 n
O4 La1 2.3240(5) . 1_555 n
O4 La1 2.3240(5) . 3_555 n
O4 La1 2.3240(5) . 5_555 n
O4 Sr1 2.3240(5) . 1_555 n
O4 Sr1 2.3240(5) . 3_555 n
O4 Sr1 2.3240(5) . 5_555 n
Sr1 La1 4.30157(30) . 2_554 n
Sr1 La1 4.30157(30) . 2_555 n
Sr1 La1 4.0252(10) . 3_555 n
Sr1 La1 4.0252(10) . 5_555 n
Sr1 La1 4.30157(30) . 6_554 n
Sr1 La1 4.30157(30) . 6_555 n
Sr1 La2 4.1185(7) . 1_545 n
Sr1 La2 4.2632(7) . 2_655 n
Sr1 La2 4.2638(7) . -1_665 n
Sr1 La2 4.1191(7) . -2_556 n
Sr1 SI 3.2311(13) . 1_555 n
Sr1 SI 3.6683(14) . 3_655 n
Sr1 SI 3.3247(15) . 5_555 n
Sr1 O1 2.7297(13) . 5_555 n
Sr1 O2 2.4946(12) . 3_655 n
Sr1 O3 2.6053(10) . 1_555 n
Sr1 O3 3.4128(10) . 5_555 n
Sr1 O3 2.4684(7) . 6_555 n
Sr1 O3 3.4128(10) . -2_556 n
Sr1 O3 2.4684(7) . -3_555 n
Sr1 O3 2.6053(10) . -4_556 n
Sr1 O4 2.3240(5) . 1_555 n
Sr1 Sr1 4.30157(30) . 2_554 n
Sr1 Sr1 4.30157(30) . 2_555 n
Sr1 Sr1 4.0252(10) . 3_555 n
Sr1 Sr1 4.0252(10) . 5_555 n
Sr1 Sr1 4.30157(30) . 6_554 n
Sr1 Sr1 4.30157(30) . 6_555 n
Sr1 Sr2 4.1190(7) . 1_545 n
Sr1 Sr2 4.2637(7) . 2_655 n
Sr1 Sr2 4.2637(7) . -1_665 n
Sr1 Sr2 4.1190(7) . -2_556 n
Sr1 O5 2.4816(6) . 4_554 n
Sr1 O5 2.607160(30) . 5_555 n
Sr1 O5 2.5911(6) . 6_554 n
Sr1 O5 2.4816(6) . -1_556 n
Sr1 O5 2.607160(30) . -2_556 n
Sr1 O5 2.5911(6) . -3_556 n
Sr2 La1 4.1190(7) . 1_565 n
Sr2 La1 4.2637(7) . 2_554 n
Sr2 La1 4.1190(7) . 3_555 n
Sr2 La1 4.2637(7) . 4_664 n
Sr2 La1 4.1190(7) . 5_665 n
Sr2 La1 4.2637(7) . 6_564 n
Sr2 La2 0.00056 . 1_555 n
Sr2 La2 3.6111(18) . -2_565 n
Sr2 La2 3.6284(18) . -2_566 n
Sr2 SI 3.7270(11) . 1_555 n
Sr2 SI 3.3165(12) . 2_554 n
Sr2 SI 3.7270(11) . 3_665 n
Sr2 SI 3.3165(12) . 4_664 n
Sr2 SI 3.7270(11) . 5_565 n
Sr2 SI 3.3165(12) . 6_564 n
Sr2 O1 2.5019(10) . 1_555 n
Sr2 O1 2.5019(10) . 3_665 n
Sr2 O1 2.5019(10) . 5_565 n
Sr2 O2 2.5507(10) . 2_554 n
Sr2 O2 2.5507(10) . 4_664 n
Sr2 O2 2.5507(10) . 6_564 n
Sr2 O3 2.8910(9) . -1_665 n
Sr2 O3 2.8910(9) . -3_565 n
Sr2 O3 2.8910(9) . -5_555 n
Sr2 Sr1 4.1190(7) . 1_565 n
Sr2 Sr1 4.2637(7) . 2_554 n
Sr2 Sr1 4.1190(7) . 3_555 n
Sr2 Sr1 4.2637(7) . 4_664 n
Sr2 Sr1 4.1190(7) . 5_665 n
Sr2 Sr1 4.2637(7) . 6_564 n
Sr2 Sr2 3.6111(18) . -2_565 n
Sr2 Sr2 3.6284(18) . -2_566 n
O5 La1 2.5911(6) . 2_555 n
O5 La1 2.607160(30) . 3_555 n
O5 La1 2.4816(6) . 4_555 n
O5 SI 1.7532(10) . 2_555 n
O5 O3 0.9459(8) . 2_555 n
O5 Sr1 2.5911(6) . 2_555 n
O5 Sr1 2.607160(30) . 3_555 n
O5 Sr1 2.4816(6) . 4_555 n
O5 O5 2.027080(20) . -4_557 n
